#------------------------------------------------------------------------------
#$Date: 2017-07-11 14:26:40 +0300 (Tue, 11 Jul 2017) $
#$Revision: 198632 $
#$URL: file:///home/coder/svn-repositories/cod/cif/4/34/49/4344943.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4344943
loop_
_publ_author_name
'Ji, Huanyao'
'Li, Xiaomin'
'Xu, Donghua'
'Zhou, Yunshan'
'Zhang, Lijuan'
'Zuhra, Zareen'
'Yang, Shaowei'
_publ_section_title
;
 Synthesis, Structure, and Photoluminescence of Color-Tunable and
 White-Light-Emitting Lanthanide Metal-Organic Open Frameworks Composed of
 AlMo6(OH)6O18(3-) Polyanion and Nicotinate.
;
_journal_name_full               'Inorganic chemistry'
_journal_paper_doi               10.1021/acs.inorgchem.6b01852
_journal_year                    2016
_chemical_formula_sum            'C8 H46 Al Eu Mo6 N Na O44'
_chemical_formula_weight         1638.03
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           2
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                104.7430(10)
_cell_angle_beta                 108.981(5)
_cell_angle_gamma                108.119(4)
_cell_formula_units_Z            2
_cell_length_a                   12.932(6)
_cell_length_b                   14.338(6)
_cell_length_c                   14.510(6)
_cell_measurement_reflns_used    7301
_cell_measurement_temperature    93(2)
_cell_measurement_theta_max      27.59
_cell_measurement_theta_min      3.11
_cell_volume                     2220.6(17)
_computing_cell_refinement       'CrystalClear (Rigaku Inc., 2008)'
_computing_data_collection       'CrystalClear (Rigaku Inc., 2008)'
_computing_data_reduction        'CrystalClear (Rigaku Inc., 2008)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      93(2)
_diffrn_detector_area_resol_mean 28.5714
_diffrn_measured_fraction_theta_full 0.976
_diffrn_measured_fraction_theta_max 0.976
_diffrn_measurement_device_type  AFC10/Saturn724+
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0371
_diffrn_reflns_av_sigmaI/netI    0.0629
_diffrn_reflns_limit_h_max       15
_diffrn_reflns_limit_h_min       -14
_diffrn_reflns_limit_k_max       17
_diffrn_reflns_limit_k_min       -17
_diffrn_reflns_limit_l_max       17
_diffrn_reflns_limit_l_min       -17
_diffrn_reflns_number            15489
_diffrn_reflns_theta_full        25.50
_diffrn_reflns_theta_max         25.50
_diffrn_reflns_theta_min         3.01
_diffrn_standards_decay_%        0
_diffrn_standards_interval_count 0
_diffrn_standards_interval_time  0
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    3.181
_exptl_absorpt_correction_T_max  0.4839
_exptl_absorpt_correction_T_min  0.3627
_exptl_absorpt_correction_type   multi-scan
_exptl_crystal_colour            Colorless
_exptl_crystal_density_diffrn    2.450
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       Block
_exptl_crystal_F_000             1584
_exptl_crystal_size_max          0.40
_exptl_crystal_size_mid          0.30
_exptl_crystal_size_min          0.27
_refine_diff_density_max         5.211
_refine_diff_density_min         -3.014
_refine_diff_density_rms         0.353
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.019
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     565
_refine_ls_number_reflns         8081
_refine_ls_number_restraints     60
_refine_ls_restrained_S_all      1.016
_refine_ls_R_factor_all          0.0915
_refine_ls_R_factor_gt           0.0836
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.1000P)²+198.0000P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.2333
_refine_ls_wR_factor_ref         0.2382
_reflns_number_gt                7044
_reflns_number_total             8081
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic6b01852_si_002.cif
_cod_data_source_block           574
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Triclinic' changed to 'triclinic'
according to
/usr/data/users/saulius/crontab/automatic-downloads/rss-feeds/ACS/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 4268 2015-11-12 08:31:59Z antanas 

The following automatic conversions were performed:

'_exptl_absorpt_correction_type' value 'multi-scans' was replaced
with the value 'multi-scan' as specified in the replacement file
'src/cod-tools/trunk/data/replacement-values/replacement_values.lst'.

Automatic conversion script
Id: cif_fix_values 5376 2017-05-30 11:51:03Z andrius 
;
_cod_original_sg_symbol_H-M      P-1
_cod_database_code               4344943
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Eu1 Eu 0.49806(7) 0.89729(6) 0.56945(6) 0.0110(2) Uani 1 1 d . . .
Mo1 Mo 0.14214(11) 0.71242(10) 0.46809(11) 0.0097(3) Uani 1 1 d . . .
Mo2 Mo 0.10426(12) 0.47870(11) 0.31954(11) 0.0107(3) Uani 1 1 d . . .
Mo3 Mo -0.04148(11) 0.26434(10) 0.35082(10) 0.0097(3) Uani 1 1 d . . .
Mo4 Mo 0.38727(13) 0.64102(11) 0.88939(12) 0.0184(4) Uani 1 1 d . . .
Mo5 Mo 0.35948(12) 0.40858(11) 0.74064(11) 0.0130(3) Uani 1 1 d . . .
Mo6 Mo 0.46854(13) 0.26825(12) 0.85139(12) 0.0187(4) Uani 1 1 d . . .
Al1 Al 0.0000 0.5000 0.5000 0.0088(12) Uani 1 2 d S . .
Al2 Al 0.5000 0.5000 1.0000 0.0079(12) Uani 1 2 d S . .
Na1 Na 0.5468(7) 0.9426(6) 0.9067(6) 0.0263(16) Uani 1 1 d . . .
O1 O 0.6531(10) 0.9291(9) 0.5119(9) 0.014(2) Uani 1 1 d U . .
O2 O 0.6307(9) 1.0212(9) 0.4101(9) 0.012(2) Uani 1 1 d U . .
O3 O 0.4086(10) 0.9088(9) 0.4063(9) 0.015(2) Uani 1 1 d U . .
O4 O 0.3517(10) 0.9436(9) 0.2672(9) 0.018(3) Uani 1 1 d . . .
O5 O 0.2912(10) 0.7603(9) 0.4866(9) 0.013(2) Uani 1 1 d . . .
O6 O 0.1486(9) 0.5629(8) 0.4946(8) 0.008(2) Uani 1 1 d U . .
O7 O 0.0651(10) 0.5980(8) 0.3308(8) 0.012(2) Uani 1 1 d . . .
O8 O -0.0233(9) 0.6178(8) 0.4791(8) 0.008(2) Uani 1 1 d . . .
O9 O 0.1789(9) 0.7638(9) 0.6175(8) 0.012(2) Uani 1 1 d . . .
O10 O 0.0875(9) 0.7973(9) 0.4317(9) 0.013(2) Uani 1 1 d . . .
O11 O -0.0577(9) 0.4166(8) 0.3532(9) 0.011(2) Uani 1 1 d . . .
O12 O 0.1075(10) 0.3624(9) 0.3579(9) 0.014(2) Uani 1 1 d U . .
O13 O 0.2531(10) 0.5378(9) 0.3401(9) 0.016(2) Uani 1 1 d . . .
O14 O 0.0228(11) 0.4118(9) 0.1857(9) 0.016(2) Uani 1 1 d . . .
O15 O -0.1226(10) 0.1921(9) 0.2184(10) 0.018(2) Uani 1 1 d . . .
O16 O 0.0167(10) 0.1878(9) 0.4014(9) 0.014(2) Uani 1 1 d . . .
O1W O 0.4372(9) 0.8490(9) 0.7064(9) 0.013(2) Uani 1 1 d U . .
O2W O 0.6436(12) 0.8439(11) 0.6759(11) 0.027(3) Uani 1 1 d . . .
O3W O 0.4707(12) 0.7242(11) 0.4557(13) 0.035(3) Uani 1 1 d . . .
O17 O 0.5519(10) 0.6412(9) 1.0070(9) 0.013(2) Uani 1 1 d . . .
O18 O 0.3497(9) 0.4772(9) 0.8960(9) 0.012(2) Uani 1 1 d . . .
O19 O 0.4296(10) 0.5628(10) 0.7891(9) 0.017(2) Uani 1 1 d . . .
O20 O 0.2377(11) 0.6004(10) 0.8084(10) 0.025(3) Uani 1 1 d U . .
O21 O 0.3801(11) 0.6781(10) 1.0236(9) 0.022(3) Uani 1 1 d . . .
O22 O 0.4594(13) 0.7654(10) 0.8952(10) 0.025(3) Uani 1 1 d . . .
O23 O 0.5301(9) 0.4447(9) 0.8842(9) 0.013(2) Uani 1 1 d . . .
O24 O 0.3301(10) 0.2862(9) 0.7731(9) 0.016(2) Uani 1 1 d . . .
O25 O 0.2115(10) 0.3801(9) 0.6633(9) 0.016(2) Uani 1 1 d . . .
O26 O 0.4222(12) 0.3836(10) 0.6541(9) 0.025(3) Uani 1 1 d . . .
O27 O 0.3992(12) 0.1495(10) 0.8573(9) 0.026(3) Uani 1 1 d . . .
O28 O 0.5217(13) 0.2425(11) 0.7581(11) 0.030(3) Uani 1 1 d . . .
N1 N 0.9017(11) 0.8673(10) 0.4231(10) 0.011(3) Uani 1 1 d U . .
C1 C 0.9286(14) 0.8979(13) 0.3502(12) 0.014(3) Uani 1 1 d . . .
H1 H 0.9832 0.8795 0.3273 0.017 Uiso 1 1 calc R . .
C2 C 0.8739(14) 0.9574(13) 0.3096(14) 0.015(3) Uani 1 1 d . . .
H2 H 0.8914 0.9806 0.2584 0.018 Uiso 1 1 calc R . .
C3 C 0.7954(15) 0.9825(12) 0.3428(13) 0.015(3) Uani 1 1 d . . .
H3 H 0.7583 1.0237 0.3159 0.018 Uiso 1 1 calc R . .
C4 C 0.7705(15) 0.9464(12) 0.4171(13) 0.012(3) Uani 1 1 d . . .
C5 C 0.8217(14) 0.8876(13) 0.4557(13) 0.013(3) Uani 1 1 d . . .
H5 H 0.8020 0.8612 0.5045 0.016 Uiso 1 1 calc R . .
C6 C 0.6759(14) 0.9681(12) 0.4496(12) 0.012(3) Uani 1 1 d . . .
C7 C 0.2508(15) 0.7625(14) 0.2481(16) 0.025(4) Uani 1 1 d . . .
H7A H 0.2369 0.7408 0.1737 0.031 Uiso 1 1 calc R . .
H7B H 0.1746 0.7550 0.2521 0.031 Uiso 1 1 calc R . .
H7C H 0.2809 0.7171 0.2782 0.031 Uiso 1 1 calc R . .
C8 C 0.3428(15) 0.8770(14) 0.3096(14) 0.018(4) Uani 1 1 d U . .
O4W O 0.3734(11) 0.9724(10) 0.9040(10) 0.025(3) Uani 1 1 d . . .
O5W O 0.7025(13) 0.8907(12) 0.8925(13) 0.036(3) Uani 1 1 d . . .
O6W O 0.6656(14) 1.1210(11) 0.9296(11) 0.034(3) Uani 1 1 d . . .
O7W O 0.0219(14) 0.2012(13) 0.8807(13) 0.040(4) Uani 1 1 d . . .
O8W O 0.1060(10) 0.3810(11) 0.8422(10) 0.025(3) Uani 1 1 d . . .
O9W O 0.7313(12) 0.5278(12) 0.8583(11) 0.033(3) Uani 1 1 d U . .
O10W O -0.3836(11) 0.3719(10) 0.3718(10) 0.024(3) Uani 1 1 d . . .
O11W O 0.7419(13) 0.7297(12) 0.9698(12) 0.035(3) Uani 1 1 d . . .
O12W O 0.0797(18) 0.7860(17) 0.9770(16) 0.062(5) Uani 1 1 d . . .
O13W O -0.0961(19) -0.0083(16) 0.755(2) 0.087(9) Uani 1 1 d . . .
O14W O 0.9457(19) 1.034(2) 1.064(2) 0.087(8) Uani 1 1 d . . .
OAW O -0.300(2) 0.686(2) 0.572(2) 0.048(5) Uani 0.70(3) 1 d P A 1
OBW O 0.092(4) 0.521(3) 1.000(3) 0.048(5) Uani 0.53(4) 1 d P B 1
OAW' O -0.316(5) 0.675(5) 0.638(5) 0.048(5) Uani 0.30(3) 1 d P A 2
OBW' O 0.158(4) 0.544(3) 1.015(3) 0.048(5) Uani 0.47(4) 1 d P B 2
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Na Na 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Al Al 0.0645 0.0514 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Eu Eu -0.1578 3.6682 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O3 Eu1 O2 74.9(4) . 2_676
O3 Eu1 O1 76.2(4) . .
O2 Eu1 O1 135.2(4) 2_676 .
O3 Eu1 O5 75.8(4) . .
O2 Eu1 O5 71.0(4) 2_676 .
O1 Eu1 O5 132.2(4) . .
O3 Eu1 O3W 82.9(5) . .
O2 Eu1 O3W 135.7(4) 2_676 .
O1 Eu1 O3W 72.2(4) . .
O5 Eu1 O3W 66.5(4) . .
O3 Eu1 O4 122.3(4) . 2_676
O2 Eu1 O4 81.8(4) 2_676 2_676
O1 Eu1 O4 85.6(4) . 2_676
O5 Eu1 O4 142.2(4) . 2_676
O3W Eu1 O4 141.7(4) . 2_676
O3 Eu1 O2W 146.3(4) . .
O2 Eu1 O2W 138.8(4) 2_676 .
O1 Eu1 O2W 75.2(4) . .
O5 Eu1 O2W 112.1(4) . .
O3W Eu1 O2W 71.8(5) . .
O4 Eu1 O2W 72.5(4) 2_676 .
O3 Eu1 O1W 138.8(4) . .
O2 Eu1 O1W 74.2(4) 2_676 .
O1 Eu1 O1W 144.4(4) . .
O5 Eu1 O1W 68.8(4) . .
O3W Eu1 O1W 101.1(5) . .
O4 Eu1 O1W 79.0(4) 2_676 .
O2W Eu1 O1W 69.7(4) . .
O3 Eu1 O3 71.5(4) . 2_676
O2 Eu1 O3 69.5(4) 2_676 2_676
O1 Eu1 O3 69.2(4) . 2_676
O5 Eu1 O3 133.7(4) . 2_676
O3W Eu1 O3 137.6(5) . 2_676
O4 Eu1 O3 50.9(4) 2_676 2_676
O2W Eu1 O3 113.5(4) . 2_676
O1W Eu1 O3 120.5(4) . 2_676
O3 Eu1 C8 96.9(5) . 2_676
O2 Eu1 C8 74.9(4) 2_676 2_676
O1 Eu1 C8 75.5(4) . 2_676
O5 Eu1 C8 145.8(4) . 2_676
O3W Eu1 C8 146.8(4) . 2_676
O4 Eu1 C8 25.5(5) 2_676 2_676
O2W Eu1 C8 92.7(5) . 2_676
O1W Eu1 C8 100.6(4) . 2_676
O3 Eu1 C8 25.4(4) 2_676 2_676
O3 Eu1 Eu1 37.4(3) . 2_676
O2 Eu1 Eu1 67.8(3) 2_676 2_676
O1 Eu1 Eu1 68.4(3) . 2_676
O5 Eu1 Eu1 107.2(3) . 2_676
O3W Eu1 Eu1 113.5(4) . 2_676
O4 Eu1 Eu1 85.0(3) 2_676 2_676
O2W Eu1 Eu1 138.3(3) . 2_676
O1W Eu1 Eu1 140.4(2) . 2_676
O3 Eu1 Eu1 34.1(3) 2_676 2_676
C8 Eu1 Eu1 59.6(4) 2_676 2_676
O10 Mo1 O5 106.7(5) . .
O10 Mo1 O7 98.0(5) . .
O5 Mo1 O7 100.2(5) . .
O10 Mo1 O9 100.4(5) . .
O5 Mo1 O9 96.3(5) . .
O7 Mo1 O9 150.5(5) . .
O10 Mo1 O8 94.2(4) . .
O5 Mo1 O8 158.3(4) . .
O7 Mo1 O8 82.3(4) . .
O9 Mo1 O8 73.6(4) . .
O10 Mo1 O6 160.9(4) . .
O5 Mo1 O6 91.6(4) . .
O7 Mo1 O6 72.9(4) . .
O9 Mo1 O6 82.5(4) . .
O8 Mo1 O6 68.4(4) . .
O14 Mo2 O13 104.9(6) . .
O14 Mo2 O12 99.5(5) . .
O13 Mo2 O12 99.2(5) . .
O14 Mo2 O7 96.9(5) . .
O13 Mo2 O7 100.2(5) . .
O12 Mo2 O7 150.3(5) . .
O14 Mo2 O11 94.2(5) . .
O13 Mo2 O11 160.3(5) . .
O12 Mo2 O11 72.4(4) . .
O7 Mo2 O11 81.9(4) . .
O14 Mo2 O6 160.0(5) . .
O13 Mo2 O6 93.9(5) . .
O12 Mo2 O6 83.8(4) . .
O7 Mo2 O6 72.7(4) . .
O11 Mo2 O6 67.8(4) . .
O15 Mo3 O16 106.2(6) . .
O15 Mo3 O9 95.9(5) . 2_566
O16 Mo3 O9 99.7(5) . 2_566
O15 Mo3 O12 101.2(5) . .
O16 Mo3 O12 97.1(5) . .
O9 Mo3 O12 151.6(5) 2_566 .
O15 Mo3 O11 97.6(5) . .
O16 Mo3 O11 155.4(5) . .
O9 Mo3 O11 83.6(4) 2_566 .
O12 Mo3 O11 71.9(4) . .
O15 Mo3 O8 162.1(5) . 2_566
O16 Mo3 O8 89.3(5) . 2_566
O9 Mo3 O8 72.1(4) 2_566 2_566
O12 Mo3 O8 85.4(4) . 2_566
O11 Mo3 O8 68.3(4) . 2_566
O22 Mo4 O20 104.8(6) . .
O22 Mo4 O21 99.9(6) . .
O20 Mo4 O21 98.4(6) . .
O22 Mo4 O19 98.4(6) . .
O20 Mo4 O19 99.2(6) . .
O21 Mo4 O19 150.5(5) . .
O22 Mo4 O17 95.9(5) . .
O20 Mo4 O17 158.8(5) . .
O21 Mo4 O17 73.3(4) . .
O19 Mo4 O17 81.9(5) . .
O22 Mo4 O18 162.1(6) . .
O20 Mo4 O18 91.7(5) . .
O21 Mo4 O18 84.0(5) . .
O19 Mo4 O18 71.9(4) . .
O17 Mo4 O18 68.3(4) . .
O25 Mo5 O26 106.1(6) . .
O25 Mo5 O24 98.4(5) . .
O26 Mo5 O24 101.8(6) . .
O25 Mo5 O19 99.0(5) . .
O26 Mo5 O19 97.6(6) . .
O24 Mo5 O19 149.1(5) . .
O25 Mo5 O18 93.6(5) . .
O26 Mo5 O18 159.0(5) . .
O24 Mo5 O18 81.8(5) . .
O19 Mo5 O18 71.9(4) . .
O25 Mo5 O23 160.6(5) . .
O26 Mo5 O23 92.7(5) . .
O24 Mo5 O23 72.7(4) . .
O19 Mo5 O23 82.7(4) . .
O18 Mo5 O23 68.4(4) . .
O27 Mo6 O28 106.6(7) . .
O27 Mo6 O24 100.4(6) . .
O28 Mo6 O24 100.5(6) . .
O27 Mo6 O21 97.3(6) . 2_667
O28 Mo6 O21 97.6(6) . 2_667
O24 Mo6 O21 149.8(5) . 2_667
O27 Mo6 O23 158.5(5) . .
O28 Mo6 O23 94.7(6) . .
O24 Mo6 O23 72.6(4) . .
O21 Mo6 O23 82.1(5) 2_667 .
O27 Mo6 O17 91.6(5) . 2_667
O28 Mo6 O17 160.5(6) . 2_667
O24 Mo6 O17 82.7(5) . 2_667
O21 Mo6 O17 72.5(5) 2_667 2_667
O23 Mo6 O17 67.7(4) . 2_667
O8 Al1 O8 180.0(7) 2_566 .
O8 Al1 O6 84.7(4) 2_566 2_566
O8 Al1 O6 95.3(4) . 2_566
O8 Al1 O6 95.3(4) 2_566 .
O8 Al1 O6 84.7(4) . .
O6 Al1 O6 180.000(1) 2_566 .
O8 Al1 O11 95.3(4) 2_566 2_566
O8 Al1 O11 84.7(4) . 2_566
O6 Al1 O11 84.3(4) 2_566 2_566
O6 Al1 O11 95.7(4) . 2_566
O8 Al1 O11 84.7(4) 2_566 .
O8 Al1 O11 95.3(4) . .
O6 Al1 O11 95.7(4) 2_566 .
O6 Al1 O11 84.3(4) . .
O11 Al1 O11 180.000(2) 2_566 .
O23 Al2 O23 180.000(4) 2_667 .
O23 Al2 O17 95.7(5) 2_667 2_667
O23 Al2 O17 84.3(5) . 2_667
O23 Al2 O17 84.3(5) 2_667 .
O23 Al2 O17 95.7(5) . .
O17 Al2 O17 180.000(3) 2_667 .
O23 Al2 O18 85.4(5) 2_667 2_667
O23 Al2 O18 94.6(5) . 2_667
O17 Al2 O18 84.4(5) 2_667 2_667
O17 Al2 O18 95.6(5) . 2_667
O23 Al2 O18 94.6(5) 2_667 .
O23 Al2 O18 85.4(5) . .
O17 Al2 O18 95.6(5) 2_667 .
O17 Al2 O18 84.4(5) . .
O18 Al2 O18 180.000(3) 2_667 .
O22 Na1 O4W 93.1(5) . .
O22 Na1 O4W 95.9(5) . 2_677
O4W Na1 O4W 84.6(5) . 2_677
O22 Na1 O5W 81.4(6) . .
O4W Na1 O5W 172.8(6) . .
O4W Na1 O5W 100.6(6) 2_677 .
O22 Na1 O6W 171.0(6) . .
O4W Na1 O6W 95.3(5) . .
O4W Na1 O6W 81.7(5) 2_677 .
O5W Na1 O6W 90.4(6) . .
O22 Na1 O1W 82.1(4) . .
O4W Na1 O1W 88.7(5) . .
O4W Na1 O1W 172.9(5) 2_677 .
O5W Na1 O1W 85.8(5) . .
O6W Na1 O1W 101.3(5) . .
O22 Na1 Na1 96.1(5) . 2_677
O4W Na1 Na1 42.3(4) . 2_677
O4W Na1 Na1 42.3(4) 2_677 2_677
O5W Na1 Na1 142.7(6) . 2_677
O6W Na1 Na1 88.0(5) . 2_677
O1W Na1 Na1 131.0(5) . 2_677
C6 O1 Eu1 135.5(10) . .
C6 O2 Eu1 137.6(10) . 2_676
C8 O3 Eu1 157.8(11) . .
C8 O3 Eu1 93.6(10) . 2_676
Eu1 O3 Eu1 108.5(4) . 2_676
C8 O4 Eu1 96.8(10) . 2_676
Mo1 O5 Eu1 152.9(6) . .
Al1 O6 Mo1 102.2(4) . .
Al1 O6 Mo2 103.6(4) . .
Mo1 O6 Mo2 90.9(4) . .
Mo2 O7 Mo1 117.5(5) . .
Al1 O8 Mo1 104.7(4) . .
Al1 O8 Mo3 102.8(4) . 2_566
Mo1 O8 Mo3 92.7(4) . 2_566
Mo3 O9 Mo1 116.0(5) 2_566 .
Al1 O11 Mo3 104.1(5) . .
Al1 O11 Mo2 104.2(5) . .
Mo3 O11 Mo2 93.7(4) . .
Mo2 O12 Mo3 117.9(6) . .
Na1 O1W Eu1 128.8(5) . .
Al2 O17 Mo4 104.4(5) . .
Al2 O17 Mo6 103.7(5) . 2_667
Mo4 O17 Mo6 92.8(4) . 2_667
Al2 O18 Mo4 103.0(4) . .
Al2 O18 Mo5 102.9(5) . .
Mo4 O18 Mo5 93.2(4) . .
Mo4 O19 Mo5 117.7(6) . .
Mo4 O21 Mo6 116.2(6) . 2_667
Mo4 O22 Na1 174.9(8) . .
Al2 O23 Mo6 104.2(5) . .
Al2 O23 Mo5 103.3(5) . .
Mo6 O23 Mo5 91.0(4) . .
Mo5 O24 Mo6 117.3(6) . .
C5 N1 C1 123.7(14) . .
N1 C1 C2 117.8(15) . .
N1 C1 H1 121.1 . .
C2 C1 H1 121.1 . .
C3 C2 C1 120.3(15) . .
C3 C2 H2 119.8 . .
C1 C2 H2 119.8 . .
C2 C3 C4 118.5(16) . .
C2 C3 H3 120.7 . .
C4 C3 H3 120.7 . .
C5 C4 C3 121.6(15) . .
C5 C4 C6 119.5(14) . .
C3 C4 C6 118.9(14) . .
C4 C5 N1 118.0(15) . .
C4 C5 H5 121.0 . .
N1 C5 H5 121.0 . .
O2 C6 O1 127.8(15) . .
O2 C6 C4 116.4(14) . .
O1 C6 C4 115.8(13) . .
C8 C7 H7A 109.5 . .
C8 C7 H7B 109.5 . .
H7A C7 H7B 109.5 . .
C8 C7 H7C 109.5 . .
H7A C7 H7C 109.5 . .
H7B C7 H7C 109.5 . .
O3 C8 O4 118.6(16) . .
O3 C8 C7 119.8(16) . .
O4 C8 C7 121.5(16) . .
O3 C8 Eu1 61.0(9) . 2_676
O4 C8 Eu1 57.7(9) . 2_676
C7 C8 Eu1 174.5(11) . 2_676
Na1 O4W Na1 95.4(5) . 2_677
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Eu1 O3 2.346(11) .
Eu1 O2 2.362(10) 2_676
Eu1 O1 2.375(11) .
Eu1 O5 2.428(11) .
Eu1 O3W 2.448(14) .
Eu1 O4 2.468(12) 2_676
Eu1 O2W 2.474(13) .
Eu1 O1W 2.536(11) .
Eu1 O3 2.539(11) 2_676
Eu1 C8 2.899(17) 2_676
Eu1 Eu1 3.967(2) 2_676
Mo1 O10 1.697(11) .
Mo1 O5 1.734(11) .
Mo1 O7 1.918(10) .
Mo1 O9 1.941(11) .
Mo1 O8 2.229(10) .
Mo1 O6 2.293(10) .
Mo2 O14 1.701(11) .
Mo2 O13 1.731(11) .
Mo2 O12 1.896(11) .
Mo2 O7 1.914(11) .
Mo2 O11 2.269(10) .
Mo2 O6 2.303(11) .
Mo3 O15 1.693(12) .
Mo3 O16 1.696(11) .
Mo3 O9 1.926(11) 2_566
Mo3 O12 1.952(11) .
Mo3 O11 2.250(11) .
Mo3 O8 2.302(11) 2_566
Mo4 O22 1.701(12) .
Mo4 O20 1.712(12) .
Mo4 O21 1.925(13) .
Mo4 O19 1.935(12) .
Mo4 O17 2.252(11) .
Mo4 O18 2.280(11) .
Mo5 O25 1.724(11) .
Mo5 O26 1.726(13) .
Mo5 O24 1.888(11) .
Mo5 O19 1.937(12) .
Mo5 O18 2.280(11) .
Mo5 O23 2.286(11) .
Mo6 O27 1.699(14) .
Mo6 O28 1.717(14) .
Mo6 O24 1.917(11) .
Mo6 O21 1.938(11) 2_667
Mo6 O23 2.269(11) .
Mo6 O17 2.278(12) 2_667
Al1 O8 1.886(10) 2_566
Al1 O8 1.886(10) .
Al1 O6 1.888(10) 2_566
Al1 O6 1.888(10) .
Al1 O11 1.907(11) 2_566
Al1 O11 1.907(11) .
Al2 O23 1.883(11) 2_667
Al2 O23 1.883(11) .
Al2 O17 1.889(11) 2_667
Al2 O17 1.889(11) .
Al2 O18 1.900(10) 2_667
Al2 O18 1.900(10) .
Na1 O22 2.375(14) .
Na1 O4W 2.400(15) .
Na1 O4W 2.401(15) 2_677
Na1 O5W 2.403(16) .
Na1 O6W 2.409(16) .
Na1 O1W 2.532(13) .
Na1 Na1 3.550(15) 2_677
O1 C6 1.24(2) .
O2 C6 1.238(19) .
O2 Eu1 2.362(10) 2_676
O3 C8 1.25(2) .
O3 Eu1 2.539(11) 2_676
O4 C8 1.26(2) .
O4 Eu1 2.468(12) 2_676
O8 Mo3 2.302(11) 2_566
O9 Mo3 1.926(11) 2_566
O17 Mo6 2.278(12) 2_667
O21 Mo6 1.938(11) 2_667
N1 C5 1.35(2) .
N1 C1 1.35(2) .
C1 C2 1.39(2) .
C1 H1 0.9500 .
C2 C3 1.36(2) .
C2 H2 0.9500 .
C3 C4 1.39(2) .
C3 H3 0.9500 .
C4 C5 1.34(2) .
C4 C6 1.53(2) .
C5 H5 0.9500 .
C7 C8 1.50(2) .
C7 H7A 0.9800 .
C7 H7B 0.9800 .
C7 H7C 0.9800 .
C8 Eu1 2.899(17) 2_676
O4W Na1 2.401(15) 2_677
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_4
O3 Eu1 O1 C6 22.0(14) . .
O2 Eu1 O1 C6 -29.1(17) 2_676 .
O5 Eu1 O1 C6 77.6(15) . .
O3W Eu1 O1 C6 108.8(15) . .
O4 Eu1 O1 C6 -102.9(15) 2_676 .
O2W Eu1 O1 C6 -175.9(15) . .
O1W Eu1 O1 C6 -167.0(13) . .
O3 Eu1 O1 C6 -53.2(14) 2_676 .
C8 Eu1 O1 C6 -79.1(15) 2_676 .
Eu1 Eu1 O1 C6 -16.5(14) 2_676 .
O2 Eu1 O3 C8 -112(3) 2_676 .
O1 Eu1 O3 C8 103(3) . .
O5 Eu1 O3 C8 -38(3) . .
O3W Eu1 O3 C8 30(3) . .
O4 Eu1 O3 C8 179(3) 2_676 .
O2W Eu1 O3 C8 71(3) . .
O1W Eu1 O3 C8 -69(3) . .
O3 Eu1 O3 C8 175(3) 2_676 .
C8 Eu1 O3 C8 176(3) 2_676 .
Eu1 Eu1 O3 C8 175(3) 2_676 .
O2 Eu1 O3 Eu1 73.0(4) 2_676 2_676
O1 Eu1 O3 Eu1 -72.4(4) . 2_676
O5 Eu1 O3 Eu1 146.7(5) . 2_676
O3W Eu1 O3 Eu1 -145.8(5) . 2_676
O4 Eu1 O3 Eu1 3.1(6) 2_676 2_676
O2W Eu1 O3 Eu1 -104.8(8) . 2_676
O1W Eu1 O3 Eu1 115.5(5) . 2_676
O3 Eu1 O3 Eu1 0.0 2_676 2_676
C8 Eu1 O3 Eu1 0.7(5) 2_676 2_676
O10 Mo1 O5 Eu1 57.5(14) . .
O7 Mo1 O5 Eu1 159.2(13) . .
O9 Mo1 O5 Eu1 -45.3(14) . .
O8 Mo1 O5 Eu1 -105.9(16) . .
O6 Mo1 O5 Eu1 -127.9(13) . .
O3 Eu1 O5 Mo1 -98.8(14) . .
O2 Eu1 O5 Mo1 -20.1(13) 2_676 .
O1 Eu1 O5 Mo1 -154.5(12) . .
O3W Eu1 O5 Mo1 172.9(15) . .
O4 Eu1 O5 Mo1 26.2(17) 2_676 .
O2W Eu1 O5 Mo1 115.8(13) . .
O1W Eu1 O5 Mo1 59.8(13) . .
O3 Eu1 O5 Mo1 -52.8(15) 2_676 .
C8 Eu1 O5 Mo1 -17.5(18) 2_676 .
Eu1 Eu1 O5 Mo1 -78.4(13) 2_676 .
O8 Al1 O6 Mo1 179.7(4) 2_566 .
O8 Al1 O6 Mo1 -0.3(4) . .
O6 Al1 O6 Mo1 6(100) 2_566 .
O11 Al1 O6 Mo1 -84.4(5) 2_566 .
O11 Al1 O6 Mo1 95.6(5) . .
O8 Al1 O6 Mo2 85.8(4) 2_566 .
O8 Al1 O6 Mo2 -94.2(4) . .
O6 Al1 O6 Mo2 -88(100) 2_566 .
O11 Al1 O6 Mo2 -178.4(4) 2_566 .
O11 Al1 O6 Mo2 1.6(4) . .
O10 Mo1 O6 Al1 -24.6(16) . .
O5 Mo1 O6 Al1 171.6(5) . .
O7 Mo1 O6 Al1 -88.1(5) . .
O9 Mo1 O6 Al1 75.5(5) . .
O8 Mo1 O6 Al1 0.2(4) . .
O10 Mo1 O6 Mo2 79.6(15) . .
O5 Mo1 O6 Mo2 -84.2(4) . .
O7 Mo1 O6 Mo2 16.0(4) . .
O9 Mo1 O6 Mo2 179.6(4) . .
O8 Mo1 O6 Mo2 104.4(4) . .
O14 Mo2 O6 Al1 25.8(15) . .
O13 Mo2 O6 Al1 -173.8(5) . .
O12 Mo2 O6 Al1 -74.9(5) . .
O7 Mo2 O6 Al1 86.8(5) . .
O11 Mo2 O6 Al1 -1.4(4) . .
O14 Mo2 O6 Mo1 -77.1(13) . .
O13 Mo2 O6 Mo1 83.4(5) . .
O12 Mo2 O6 Mo1 -177.8(4) . .
O7 Mo2 O6 Mo1 -16.0(4) . .
O11 Mo2 O6 Mo1 -104.3(4) . .
O14 Mo2 O7 Mo1 -175.7(6) . .
O13 Mo2 O7 Mo1 -69.1(7) . .
O12 Mo2 O7 Mo1 60.9(12) . .
O11 Mo2 O7 Mo1 91.0(6) . .
O6 Mo2 O7 Mo1 21.9(5) . .
O10 Mo1 O7 Mo2 175.2(6) . .
O5 Mo1 O7 Mo2 66.6(7) . .
O9 Mo1 O7 Mo2 -56.5(12) . .
O8 Mo1 O7 Mo2 -91.6(6) . .
O6 Mo1 O7 Mo2 -21.9(5) . .
O8 Al1 O8 Mo1 140(100) 2_566 .
O6 Al1 O8 Mo1 -179.7(5) 2_566 .
O6 Al1 O8 Mo1 0.3(5) . .
O11 Al1 O8 Mo1 96.5(5) 2_566 .
O11 Al1 O8 Mo1 -83.5(5) . .
O8 Al1 O8 Mo3 44(100) 2_566 2_566
O6 Al1 O8 Mo3 83.9(4) 2_566 2_566
O6 Al1 O8 Mo3 -96.1(4) . 2_566
O11 Al1 O8 Mo3 0.1(4) 2_566 2_566
O11 Al1 O8 Mo3 -179.9(4) . 2_566
O10 Mo1 O8 Al1 171.9(5) . .
O5 Mo1 O8 Al1 -24.0(15) . .
O7 Mo1 O8 Al1 74.3(5) . .
O9 Mo1 O8 Al1 -88.5(5) . .
O6 Mo1 O8 Al1 -0.2(4) . .
O10 Mo1 O8 Mo3 -84.1(5) . 2_566
O5 Mo1 O8 Mo3 80.0(13) . 2_566
O7 Mo1 O8 Mo3 178.4(4) . 2_566
O9 Mo1 O8 Mo3 15.5(4) . 2_566
O6 Mo1 O8 Mo3 103.8(4) . 2_566
O10 Mo1 O9 Mo3 70.5(7) . 2_566
O5 Mo1 O9 Mo3 178.8(6) . 2_566
O7 Mo1 O9 Mo3 -57.3(12) . 2_566
O8 Mo1 O9 Mo3 -20.8(5) . 2_566
O6 Mo1 O9 Mo3 -90.5(6) . 2_566
O8 Al1 O11 Mo3 0.1(4) 2_566 .
O8 Al1 O11 Mo3 -179.9(4) . .
O6 Al1 O11 Mo3 -84.0(5) 2_566 .
O6 Al1 O11 Mo3 96.0(5) . .
O11 Al1 O11 Mo3 -178(100) 2_566 .
O8 Al1 O11 Mo2 -97.5(5) 2_566 .
O8 Al1 O11 Mo2 82.5(5) . .
O6 Al1 O11 Mo2 178.4(4) 2_566 .
O6 Al1 O11 Mo2 -1.6(4) . .
O11 Al1 O11 Mo2 85(100) 2_566 .
O15 Mo3 O11 Al1 168.3(5) . .
O16 Mo3 O11 Al1 -26.1(13) . .
O9 Mo3 O11 Al1 73.2(5) 2_566 .
O12 Mo3 O11 Al1 -92.3(5) . .
O8 Mo3 O11 Al1 -0.1(4) 2_566 .
O15 Mo3 O11 Mo2 -86.0(5) . .
O16 Mo3 O11 Mo2 79.6(11) . .
O9 Mo3 O11 Mo2 178.9(4) 2_566 .
O12 Mo3 O11 Mo2 13.4(4) . .
O8 Mo3 O11 Mo2 105.6(4) 2_566 .
O14 Mo2 O11 Al1 -169.5(5) . .
O13 Mo2 O11 Al1 24.6(16) . .
O12 Mo2 O11 Al1 91.8(5) . .
O7 Mo2 O11 Al1 -73.1(5) . .
O6 Mo2 O11 Al1 1.4(4) . .
O14 Mo2 O11 Mo3 84.9(5) . .
O13 Mo2 O11 Mo3 -80.9(14) . .
O12 Mo2 O11 Mo3 -13.7(4) . .
O7 Mo2 O11 Mo3 -178.7(4) . .
O6 Mo2 O11 Mo3 -104.1(4) . .
O14 Mo2 O12 Mo3 -73.4(7) . .
O13 Mo2 O12 Mo3 179.6(6) . .
O7 Mo2 O12 Mo3 49.3(12) . .
O11 Mo2 O12 Mo3 18.0(5) . .
O6 Mo2 O12 Mo3 86.6(6) . .
O15 Mo3 O12 Mo2 76.3(7) . .
O16 Mo3 O12 Mo2 -175.6(6) . .
O9 Mo3 O12 Mo2 -49.6(13) 2_566 .
O11 Mo3 O12 Mo2 -18.2(5) . .
O8 Mo3 O12 Mo2 -86.9(6) 2_566 .
O22 Na1 O1W Eu1 -147.4(6) . .
O4W Na1 O1W Eu1 119.2(6) . .
O4W Na1 O1W Eu1 139(4) 2_677 .
O5W Na1 O1W Eu1 -65.5(7) . .
O6W Na1 O1W Eu1 24.1(7) . .
Na1 Na1 O1W Eu1 121.4(6) 2_677 .
O3 Eu1 O1W Na1 -136.6(6) . .
O2 Eu1 O1W Na1 -93.8(6) 2_676 .
O1 Eu1 O1W Na1 56.7(9) . .
O5 Eu1 O1W Na1 -169.1(7) . .
O3W Eu1 O1W Na1 131.6(6) . .
O4 Eu1 O1W Na1 -9.3(6) 2_676 .
O2W Eu1 O1W Na1 65.9(6) . .
O3 Eu1 O1W Na1 -40.0(7) 2_676 .
C8 Eu1 O1W Na1 -23.0(7) 2_676 .
Eu1 Eu1 O1W Na1 -77.4(7) 2_676 .
O23 Al2 O17 Mo4 -94.6(5) 2_667 .
O23 Al2 O17 Mo4 85.4(5) . .
O17 Al2 O17 Mo4 -8(100) 2_667 .
O18 Al2 O17 Mo4 -179.4(5) 2_667 .
O18 Al2 O17 Mo4 0.6(5) . .
O23 Al2 O17 Mo6 1.9(5) 2_667 2_667
O23 Al2 O17 Mo6 -178.1(5) . 2_667
O17 Al2 O17 Mo6 88(100) 2_667 2_667
O18 Al2 O17 Mo6 -82.9(5) 2_667 2_667
O18 Al2 O17 Mo6 97.1(5) . 2_667
O22 Mo4 O17 Al2 -171.8(6) . .
O20 Mo4 O17 Al2 20.3(17) . .
O21 Mo4 O17 Al2 89.6(6) . .
O19 Mo4 O17 Al2 -74.2(6) . .
O18 Mo4 O17 Al2 -0.5(4) . .
O22 Mo4 O17 Mo6 83.2(5) . 2_667
O20 Mo4 O17 Mo6 -84.6(15) . 2_667
O21 Mo4 O17 Mo6 -15.3(4) . 2_667
O19 Mo4 O17 Mo6 -179.1(5) . 2_667
O18 Mo4 O17 Mo6 -105.4(4) . 2_667
O23 Al2 O18 Mo4 83.2(5) 2_667 .
O23 Al2 O18 Mo4 -96.8(5) . .
O17 Al2 O18 Mo4 179.4(5) 2_667 .
O17 Al2 O18 Mo4 -0.6(5) . .
O18 Al2 O18 Mo4 -34(100) 2_667 .
O23 Al2 O18 Mo5 179.7(5) 2_667 .
O23 Al2 O18 Mo5 -0.3(5) . .
O17 Al2 O18 Mo5 -84.1(5) 2_667 .
O17 Al2 O18 Mo5 95.9(5) . .
O18 Al2 O18 Mo5 62(100) 2_667 .
O22 Mo4 O18 Al2 29.7(19) . .
O20 Mo4 O18 Al2 -172.1(6) . .
O21 Mo4 O18 Al2 -73.9(5) . .
O19 Mo4 O18 Al2 88.8(5) . .
O17 Mo4 O18 Al2 0.5(4) . .
O22 Mo4 O18 Mo5 -74.3(17) . .
O20 Mo4 O18 Mo5 83.9(5) . .
O21 Mo4 O18 Mo5 -177.9(5) . .
O19 Mo4 O18 Mo5 -15.2(4) . .
O17 Mo4 O18 Mo5 -103.5(5) . .
O25 Mo5 O18 Al2 172.8(5) . .
O26 Mo5 O18 Al2 -26.8(16) . .
O24 Mo5 O18 Al2 74.8(5) . .
O19 Mo5 O18 Al2 -88.9(5) . .
O23 Mo5 O18 Al2 0.3(4) . .
O25 Mo5 O18 Mo4 -83.1(5) . .
O26 Mo5 O18 Mo4 77.4(15) . .
O24 Mo5 O18 Mo4 178.9(5) . .
O19 Mo5 O18 Mo4 15.2(4) . .
O23 Mo5 O18 Mo4 104.4(4) . .
O22 Mo4 O19 Mo5 -175.0(7) . .
O20 Mo4 O19 Mo5 -68.4(7) . .
O21 Mo4 O19 Mo5 57.3(13) . .
O17 Mo4 O19 Mo5 90.1(6) . .
O18 Mo4 O19 Mo5 20.4(5) . .
O25 Mo5 O19 Mo4 70.4(7) . .
O26 Mo5 O19 Mo4 178.2(7) . .
O24 Mo5 O19 Mo4 -53.1(12) . .
O18 Mo5 O19 Mo4 -20.4(5) . .
O23 Mo5 O19 Mo4 -90.0(6) . .
O22 Mo4 O21 Mo6 -73.1(8) . 2_667
O20 Mo4 O21 Mo6 -179.8(7) . 2_667
O19 Mo4 O21 Mo6 54.3(14) . 2_667
O17 Mo4 O21 Mo6 20.2(6) . 2_667
O18 Mo4 O21 Mo6 89.3(6) . 2_667
O20 Mo4 O22 Na1 49(9) . .
O21 Mo4 O22 Na1 -53(8) . .
O19 Mo4 O22 Na1 151(8) . .
O17 Mo4 O22 Na1 -127(8) . .
O18 Mo4 O22 Na1 -154(7) . .
O4W Na1 O22 Mo4 -12(9) . .
O4W Na1 O22 Mo4 73(8) 2_677 .
O5W Na1 O22 Mo4 172(8) . .
O6W Na1 O22 Mo4 146(7) . .
O1W Na1 O22 Mo4 -101(8) . .
Na1 Na1 O22 Mo4 30(9) 2_677 .
O23 Al2 O23 Mo6 -159(100) 2_667 .
O17 Al2 O23 Mo6 1.9(5) 2_667 .
O17 Al2 O23 Mo6 -178.1(5) . .
O18 Al2 O23 Mo6 85.8(5) 2_667 .
O18 Al2 O23 Mo6 -94.2(5) . .
O23 Al2 O23 Mo5 -65(100) 2_667 .
O17 Al2 O23 Mo5 96.4(5) 2_667 .
O17 Al2 O23 Mo5 -83.6(5) . .
O18 Al2 O23 Mo5 -179.7(5) 2_667 .
O18 Al2 O23 Mo5 0.3(5) . .
O27 Mo6 O23 Al2 13.8(16) . .
O28 Mo6 O23 Al2 -173.0(6) . .
O24 Mo6 O23 Al2 87.4(6) . .
O21 Mo6 O23 Al2 -76.0(6) 2_667 .
O17 Mo6 O23 Al2 -1.7(4) 2_667 .
O27 Mo6 O23 Mo5 -90.1(14) . .
O28 Mo6 O23 Mo5 83.0(6) . .
O24 Mo6 O23 Mo5 -16.6(4) . .
O21 Mo6 O23 Mo5 -179.9(5) 2_667 .
O17 Mo6 O23 Mo5 -105.7(4) 2_667 .
O25 Mo5 O23 Al2 -23.3(16) . .
O26 Mo5 O23 Al2 170.4(6) . .
O24 Mo5 O23 Al2 -88.1(6) . .
O19 Mo5 O23 Al2 73.1(5) . .
O18 Mo5 O23 Al2 -0.3(4) . .
O25 Mo5 O23 Mo6 81.6(15) . .
O26 Mo5 O23 Mo6 -84.7(5) . .
O24 Mo5 O23 Mo6 16.8(4) . .
O19 Mo5 O23 Mo6 178.0(5) . .
O18 Mo5 O23 Mo6 104.6(4) . .
O25 Mo5 O24 Mo6 175.1(7) . .
O26 Mo5 O24 Mo6 66.5(8) . .
O19 Mo5 O24 Mo6 -61.2(12) . .
O18 Mo5 O24 Mo6 -92.5(6) . .
O23 Mo5 O24 Mo6 -22.6(6) . .
O27 Mo6 O24 Mo5 -178.1(7) . .
O28 Mo6 O24 Mo5 -68.8(8) . .
O21 Mo6 O24 Mo5 57.1(14) 2_667 .
O23 Mo6 O24 Mo5 22.8(6) . .
O17 Mo6 O24 Mo5 91.6(7) 2_667 .
C5 N1 C1 C2 3(2) . .
N1 C1 C2 C3 0(2) . .
C1 C2 C3 C4 -1(2) . .
C2 C3 C4 C5 0(2) . .
C2 C3 C4 C6 -176.1(14) . .
C3 C4 C5 N1 2(2) . .
C6 C4 C5 N1 178.1(14) . .
C1 N1 C5 C4 -3(2) . .
Eu1 O2 C6 O1 9(3) 2_676 .
Eu1 O2 C6 C4 -171.8(10) 2_676 .
Eu1 O1 C6 O2 14(3) . .
Eu1 O1 C6 C4 -165.1(10) . .
C5 C4 C6 O2 -178.8(15) . .
C3 C4 C6 O2 -3(2) . .
C5 C4 C6 O1 0(2) . .
C3 C4 C6 O1 176.3(14) . .
Eu1 O3 C8 O4 -172.7(19) . .
Eu1 O3 C8 O4 3.0(15) 2_676 .
Eu1 O3 C8 C7 11(4) . .
Eu1 O3 C8 C7 -173.8(13) 2_676 .
Eu1 O3 C8 Eu1 -176(3) . 2_676
Eu1 O4 C8 O3 -3.1(16) 2_676 .
Eu1 O4 C8 C7 173.6(13) 2_676 .
O22 Na1 O4W Na1 95.6(5) . 2_677
O4W Na1 O4W Na1 0.000(1) 2_677 2_677
O5W Na1 O4W Na1 137(5) . 2_677
O6W Na1 O4W Na1 -81.1(5) . 2_677
O1W Na1 O4W Na1 177.6(5) . 2_677
